Presentation on theme: "Material removal: etching processes"— Presentation transcript:
1 Material removal: etching processes Etching is done either in “dry” or “wet” methods:Wet etching uses liquid etchants with wafers immersed in etchant solution.Wet etch is cheap and simple, but hard to control (not reproducible), not popular for Nano for pattern transfer purpose.Dry etching uses gas phase etchants in a plasma, both chemical and physical (sputtering process).Dry plasma etch can be used for many dielectric materials and some metals (Al, Ti, Cr, Ta, W…).For other metals, ion milling (Ar+) can be used, but with low etching selectivity. (as a result, for metals that cannot be dry-etched, it is better to pattern them using liftoff)Etching selectivity:The ratio of etching rates between different materials, usually the higher the better. Generally, chemical etching has high selectivity, physical etching (sputtering, milling) has low selectivity.ECE 730: Fabrication in the nanoscale: principles, technology and applicationsInstructor: Bo Cui, ECE, University of Waterloo;Textbook: Nanofabrication: principles, capabilities and limits, by Zheng Cui
2 Basic concepts Etching is consisted of 3 processes: Mass transport of reactants (through a boundary layer) to the surface to be etchedReaction between reactants and the film to be etched at the surfaceMass transport of reaction products from the surface through the surface boundary layer
3 Types of etching processes: isotropic vs. anisotropic Generally speaking, chemical process (wet etch, plasma etch) leads to isotropic etch; whereas physical process (directional energetic bombardment) leads to anisotropic etch.Isotropic:Best to use with large features when sidewall slope does not matter, and to undercut the mask (for easy liftoff).Large critical dimension (CD, i.e. feature size) loss, generally not for nano-fabrication.Quick, easy, and cheap.Anisotropic:Best for making small features with vertical sidewalls, preferred pattern transfer method for nano-fabrication and some micro-fabrication.Typically more costly.
4 Wet etching Etching is only chemical: great selectivity Very easy and fast (μm/min)Under etching, good for undercut (liftoff), but not well suited for nanostructures.Poor process control, not well reproducible.Etching rate:The etch rate can be controlled by any of the three serial processes (reactants transport to the surface, reaction, reaction products transport from the surface).Preference is to have reaction rate controlled process becauseEtch rate can be increased by temperatureGood control over reaction rate – temperature of a liquid is easy to controlMass transport control will result in non-uniform etch rate: edge etches faster.Etchant is stirred to minimize boundary layer and make etching more uniform.
5 Isotropic wet etching (silicon dioxide) Etch is isotropic and easily controlled by dilution of HF in H2O.Thermally grown oxide etches at120nm/min in 6H2O:1HF~1 m/min in 49 wt% HF (i.e. undiluted HF).Faster etch rate for doped or deposited oxide.High etch selectivity (SiO2/Si) > 100Buffered HF (BHF) or buffered oxide etchant (BOE) provides consistent etch ratesIn regular HF etches, HF is consumed and the etch rate drops.Serious process control issue.HF buffered with NH4F to maintain HF concentration 6NH4F:1HFNH4F→NH3↑+ HF
6 Isotropic etch (silicon) Silicon is etched by nitric acid and hydrofluoric acid mixturesUse oxidant HNO3 to oxidize silicon to form silicon dioxide, followed by HF etch of silicon dioxide.Excess nitric acid results in a lot of silicon dioxide formation and etch rate becomes limited by HF removal of oxide (polishing).CH3COOH or H2O can be added as diluent, but etch differently (acetic acid does not reduce oxidization power of the nitric acid, but water does).H2O2 (oxidant) and HF mixture can also etch Si.Si + HNO3 + 6HF → H2SiF6 + HNO2 + H2O +H2Topology of etched Si surfacespolishSi iso-etch curves using CH3COOH or H2O diluentMarc Madou, “Fundamentals of microfabrication”, 1997 page
7 An-isotropic wet etching (silicon) Orientation selective etch of silicon occur in hydroxide solutions because of the close packing of some orientations relative to other orientationsDensity of planes: <111> > <110> > <100>Etch rate: R(111) < R(110) < R(100)<100> direction etches faster than <111> direction, with etch rateR(100)= 100 R(111)It is reaction rate limitedMost useful for Si3N4 membrane fabrication (etch through Si wafer thickness, stop at nitride).Etch “stops” at (111) direction(100) Silicon waferEtch mask: SiO2 or Si3N4 or Cr/AuPopular etchant:KOH, TMAH(tetra methyl ammonium hydroxide)
9 50H3PO4:20H2O:1HNO3:1CH3COOH Isotropic etching (aluminum) Aluminum etches in water, phosphoric, nitric and acetic acid mixtures.Converts Al to Al2O3with nitric acid (evolves H2).Dissolve Al2O3 in phosphoric acid.Gas evolution leading to bubbles.Local etch rate goes down where bubble is formed, leading to non-uniformity.Al can also be etched in diluted HCl, HNO3, H2SO4, NaOH, KOH, but less controllable (etch oxide slowly and uncontrollablly, then once oxide all etched away, etch Al metal very fast).
10 Isotropic wet chemical etch: summary EtchantEtchesDoesn't etchH3PO4(19), Hac(1), HNO3(1), H2O (2)Al, SiN, MSiO2, Si, PRHF, BOE (HF, NH4F)SiO2, MSi, SiN, AuH2SO4(3), H2O2(1) pirahnaOrganics, MSi, SiO2, SiNI2(I),KI(2),H2O(10)Au, MSi, SiO2, SiN, M, PRNH4OH(5), H2O2(1)Polymers, AlSi, SiO2, SiN, MHNO3(64), NH4F(3),H2O(33)Si, MSiN, PRHCl(3), HNO3(1) aqua regiaall MM: metal; PR: photoresist
11 Wet “etch” for wafer cleaning Solvent cleaning: acetone, then methanol, then iso-propanol (2-propanol).Pirahna: H2SO4 : H2O2 = 3 : 1, remove organic and metals, can heat to >60oC.RCA clean: (all three steps are needed for thermal oxidation or LPCVD nitride)H2O2:NH4OH:H2O=1:1:5, 80oC for 10min. (remove organics and particles)H2O2:HCl:H2O=1:1:5, 80oC for 10min. (remove metals)HF:H2O=1:50, 30sec (for Si, remove native oxide and contaminants on top).Usually, only the first step is enough for such as nanoimprint mold fabrication.
12 Dry (plasma) etching Plasma react adsorb surface Directional etching due to presence of ionic species in plasma and (self-) biased electric field. (The self-bias electric field is not applied externally, but is created spontaneously in RF plasma)Two components existed in plasmaIonic species results in directional etching.Chemical reactive species results in high etch selectivity.Control of the ratio of ionic/reactive components in plasma can modulate the dry etching rate and etching profile.Neutrals (etchant gas)IonsFree radicalsadsorbreactsurfaceGaseous productsPlasmaPlasma consists of: ionized atoms/molecules, free electrons, free radicals (neutral).
13 DC plasma (glow discharge) Why self-bias?J is flux of ions/electrons that hit the electrodes, n is number density, v is velocity.Structure of glow discharge in a DC diode systemElectrons move much faster than ions, thus in the plasma region there are fewer electrons; i.e. the plasma is positively self-biased with respect to the electrodes.DC glow discharge is used for sputter deposition, sputter cleaning, or ion beam etching/milling (ion source in triode configuration).Voltage distribution in equilibrium
14 RF plasma (RF: radio frequency) Due to blocking capacitor, electrons build up on the cathode, but not on anode (grounded). So large self-bias only near cathode.Plasma(13.56 MHz)If BOTH electrodes are blocked by a capacitor:Relative voltage drop near each electrode depends on its area A. In theory, V(A)-4; but experimentally V(A)-2.Thus if connect anode to chamber wall (very large A), DC voltage drop near cathode will be very high.VDC: self-bias of cathodeVP: plasma potentialTime-averaged potential distributionIn a plasma, electrons and ions are NOT in thermal equilibrium.Electrons don’t lose energy efficiently by collision due to the huge mass difference, so electrons are very “hot” with energy 1-10eV (equivalent to K); to a certain degree, plasma is very reactive because the electrons are “hot”, as if the reactants were heated.(ions lose energy by collision, so they are “cold” with energy ~0.04eV)
15 RF plasma chemistry CF4 plasma RF plasma is more widely used for dry etching pattern transfer in nanofabrication than DC plasma. (RF plasma is also used for thin film deposition as in plasma enhanced CVD (PECVD) and RF-sputtering)CF4 plasmaphoton (glow)
16 RF plasma chemistryIn a plasma, reactive neutral chemical species (free radicals, e.g. F atoms or molecular species) are mainly responsible for the chemical reaction partly due to their great numbers compared to ions.Those free radicals are more abundant than ions because: 1) they are generated at lower threshold energy (e.g. <8eV; in comparison, Ar is ionized at 15.7eV); and 2) they (uncharged radicals) have longer lifetime in the plasma.The neutral radicals arrive at cathode surface by diffusion (so non-directional).Charged ions are accelerated to the cathode due to self-bias. (Unless with very high energy of >100eV as in ion beam etching), ion itself doesn’t contribute significantly to the chemical reaction mostly due to its very low concentration, but ion bombardment can greatly enhance the chemical reaction in reactive ion etching (RIE).In RIE, ion energy is low ~10eV due to collision energy loss. The name reactive “ion” etching is very misleading since ions don’t contribute directly to etching.
18 Types of dry etching processes (e.g. XeF2 gas etch Si even without plasma)(e.g. ion beam etching/milling using Ar+)RIE is most popular for nanofabrication.Plasma etching can be used to remove a layer such as photoresist residue.
19 High density plasma etching Ion milling & Sputter etching Plasma etching mechanismChemical etching: free radicals react with material to be removed. E.g. plasma etching at high pressure close to 1Torr.Physical etching or sputtering: ionic species, accelerated by the built-in electric field (self-bias), bombard the materials to be removed. E.g. sputter cleaning using Ar gas in sputter deposition system.Ion enhanced etching: combined chemical and physical process, higher material removal rate than each process alone. E.g. reactive ion etching (RIE), which is the most widely used dry etching technique.Physical ProcessChemical ProcessReactive Ion etchingHigh density plasma etchingIon milling & Sputter etchingWet etchingPlasma etchingPressureEnergy (power)SelectivityAnisotropicity
20 Chemical etchFree radicals are electrically neutral species that have incomplete outer shells e.g. CF3and FFree radicals react with film to be etched and form volatile by-products.Mass transport of reactive species from the gas stream to the reaction surface, reaction takes place at the surface, followed by mass transport of reaction products back to the gas stream.Pure chemical etch is isotropic or nearly isotropic, and the etching profile depends on arrival angles and sticking coefficients of free radicals. Free radicals (un-charged) in plasma systems have isotropic arrival angles and low sticking coefficients (bounce back for under-etch).
21 Si etching with F radicals Isotropic etchingXeF2 or SF6 plasma, no side-wall passivation, so large undercut profile.
22 Plasma etch methods for various films Most reactant gasses contain halogens: Cl, F, Br, or IExact choice of reactant gasses to etch each specific film depends onAbility to form volatile by-products that can be removed by pumpingEtch selectivity to resist and underlying filmsAnisotropicityBoiling points are good indicators of volatility of speciesLower boiling point, higher tendency to evaporate.High boiling point may need etching at elevated tempartures.
23 Physical etch component in a plasma etch system (much less important than chemical etch)Ionic species are accelerated towards each electrode by built-in self-bias.The ionic species such as Cl2+, CF4+, CF3+ (or Ar+ in a purely physical sputter etch) strike the wafer surface and remove the material to be etched.Physical etch is directional and non- selective (sputter yield does not vary much for different materials).
24 Pure physical etch: sputter etching system Ar plasmaUse inert gas, usually for in-situ substrate surface cleaning before sputter deposition.Self-bias few 100V, but low ion energy (order 10V) due to collision energy loss.Therefore, very low mill rate in a sputter system, for surface cleaning only.
25 Ion beam etching (IBE) system: triode configuration DC plasma ion beam sourceRF plasma ion beam sourceElectron beam is first generated by hot filament.Ions is generated by electron bombardment, then accelerated to bombard the substrate.Can be pure physical milling or chemical assisted.Used for milling metals that cannot be plasma-etched.Plasma is involved to generate ion beam (but typically not considered as plasma etching).Low pressure ~10-4Torr, so large mean free path and less energy loss due to collision.High acceleration voltage (>1kV), leading to mill rate ~10-30nm/min.Physical milling when using heavy inert gases (Ar).CAIBE: chemical assisted ion beam etching, introduce chemical etching component by adding reactive gases (O2, Cl2).Unlike RIE, ions are responsible for etching; and the etch product can be non-volatile.
26 Ion beam etching (IBE) issues Purely physical sputtering process – poor selectivity and high anisotropicHigh ion energy (>500eV)Issues:Physical or radiation damageRe-depositionFaceting (sputter yield is a function of incident angle)Reactive IBE (RIBE), chemically assisted IBE (CAIBE)Increase in selectivity by chemical etchFor RIBE, reactive gases are introduced into plasma region, so ionized.For CAIBE, reactive gases are introduced into lower chamber, so not ionized. (some ionized by Ar+ bombardment)(since non-volatile)(also exist for RIE)
27 Ion enhanced plasma etch (IEE): chemical etch assisted by physical bombardmentIEE is an anisotropic and highly selective etching process.Reactive ion etch (RIE) is the most popular IEE.Ion bombardment can enhance one of the following steps during chemical etch: surface adsorption, etching reaction, by-product formation, by-product removal (inhibitor layer) and removal of un-reacted etchants.Example: formation of inhibitor layer which consists of polymer formed from CHF3 during RIE of SiO2.
28 Reactive ion etch (RIE) Schematic RIE processAnisotropic etching with vertical sidewalla) Ion sputtering, b) reactive etching, c) radical formation, d) radical etching(most important)Etching maskThe high anisotropy in RIE is due to the directional nature of the ion bombardment.High selectivity arises from the chemical interactions.Volatile product of etching prevent redeposition.Intensively used in the microelectronic industry.Well known for semiconductors and dielectrics.OK for few metals : Al (form AlCl3), Cu (CuCl2), Ti (TiFx, TiCl4), W (WF6), Cr (CrO2Cl2).
29 RIE: first proof of etching mechanism XeF2XeF2+Ar+Ar+Silicon etch rate (Å/min)Time (sec)Gas phase etch, NO plasmaVery slow etch when pure chemical or physical etch aloneg: gas, p: ?, s: solidNote: XeF2 gas can etch Si even without plasma
30 Anisotropy due to ion bombardment Anisotropic etch with vertical sidewall is desired for micro- and nano-fabrication.But directional ion bombardment doesn’t always lead to noticeable anisotropic etch.For instance, SF6 etch of Si is pretty isotropic with large undercut like wet etch.To achieve anisotropy, there are two mechanisms:Energy-driven anisotropy: bombardment by ions disrupts an un-reactive substrate and causes damages such as dangling bonds and dislocations, resulting in a substrate more reactive towards etchant species (electrons or photons can also induce surface activation). E.g. CAIBE (chemical assisted ion beam etching)Inhibitor-driven anisotropy: in this case etching leads to the production of a surface covering agent (a passivation/inhibition layer). Ion bombardment removes this layer from horizontal surface (vertical surface - sidewall remain passivated), and reaction with neutrals proceed on these un-passivated surfaces only. E.g. RIE of SiO2 using CHF3 gases to form fluorocarbon passivation layer.
31 Etching profile: sidewall passivation by inhibitor deposition High inhibitor deposition rateLow inhibitor deposition rateInhibitor deposits both on sidewall and on bottom.Inhibitor on bottom can be removed by ion bombardment.So only sidewall is protected by inhibitor, leading to anisotropic etch without undercut.Nearly vertical sidewalls is possible.Fluoropolymer (like Teflon) in CHF3 or CF4+H2 RIE of Si or SiO2 is the inhibitor.Teflon
32 Parallel plate etchers (regular RIE, low density plasma) Both chemical reaction and physical sputtering process occur.Plasma etch mode:Pressure: 100 – 1000mTorrVoltage drop (self-bias) VReactive ion etch (RIE) mode:Pressure: mTorrVoltage drop VRIE has high voltage drop, so is more directional/anisotropic than plasma etch.This is sputter deposition configuration; for etching, the blocking capacitor… should be connected to the bottom electrode on top of which sit the wafers.Parallel plate etcher is low density plasma system: the reactive species and ions have very low density, leading to low etch rate.
33 High density plasma system Inductively coupled plasma (ICP)(four systems at Waterloo)Electron cyclotron resonance plasma(less common)ICP power(for dense plasma)plasmaRF bias power(similar to RIE, parallel plate)High magnetic field in the coil, so electrons move in circles with long path, leading to higher collision and ionization probability.Plasma density ions/cm3; may have low operation pressure mTorr.Independent control of RF bias (ion energy, directionality) and ion density (plasma density, chemical etching rate).High etching rate than RIE, but may be less anisotropic due to increased chemical etching.ICP etcher can be used as a pure RIE etcher by turning off the ICP component.
34 RIE/plasma etch gasesMost lab systems have only fluorine-based gases (SF6, CF4, CHF3) since they are relatively safe; chlorine-based gases are corrosive. Most RIE has Ar and O2 gas, some has H2 and He.
35 Plasma etching (silicon dioxide) CF4 etch is isotropic; anisotropic etching can be achieved by adding H2 to reduce F free radicals.Use of CHF3 or C2F6 results in more C-F (Teflon) polymer deposition on sidewalls.High bias voltage ( eV) can enhance vertical etch rate.In general, use of O2 to increase F concentration and H2 to reduce F concentration. (O reacts with CF3and CF2 and hence reduce the recombination rate of F)Reduction of F/C ratio of the etch gas improves selectivity of SiO2 over Si.Polymer inhibitor on sidewalls needs to be removed with O2 or CF4.Effect of C/F ratioInhibitor: Teflon like fluorocarbon polymer
36 Plasma/RIE etching (silicon) Fluorine based chemistry (CF4, NF3 and SF6) tend to be isotropic.When anisopicity is not important, SF6/O2 is a good chemistry for high selectivity.When anisotropicity is desired, start with CF4/H2 and followed by CF4/O2 (undercutting may occur).Chlorine based chemistry (Cl2, HCl, SiCl4, BCl3) result in anisotropic and selective etching (etch rate lower than F chemistry).Etch rate increased by ion bombardmentCan be anisotropic without polymer inhibitor formationSelectivity to oxide is high (100:1)Anisotropicity enhanced by adding small amount of O2Bromine based chemistry (HBr, Br2) are similar to chlorine based etchants (etch rate slower than F or Cl).Anisotropic and selective to oxide without polymer inhibitorAdding O2 promotes inhibitor formation (forming SiO2 from Si and removal of C from resist erosion
37 Plasma/RIE etching (aluminum) Presence of native oxide Al2O3 on Al surface requires a breakthrough etch before the main etch.Use Ar sputterUse BCl3, SiCl4, CCl4 or BBr3 to scavenge O2 & H2OFluorine is not used because AlF3 is not volatile.Cl2 etches Al isotropically.For anisotropic etching, sidewall inhibitor formation is neededCHCl3, CFCl3, CCl4Al/Cu alloys are used in interconnects but Cu does not etch in Cl.Etch requires ion bombardment or high temperatureCorrosion of Al line occurs when exposed to ambient because Cl on sidewall and resist react with water to form HCl which etches Al. To passivate Al surface after etch before exposure to atmosphereHeat wafer to oC to drive-off ClBury Cl with CHF3 polymer and remove the polymer laterExpose to F ambient such as SF6 plasma to replace Cl with FO2 plasma followed by DI water rinse
38 Deep Si etch: ICP - “BOSCH” process Alternating etch and (inhibitor) deposition step.SF6 etch 5-13 sec; followed by C4F8 fluorocarbon polymer deposition 5-10 sec.Etch rate several 𝝁m/min, capable of etching several hundred 𝝁m with vertical walls.Side wall is rough, depending on cycle times (longer cycle, rougher).More popular for MEMS, less common for nano-fabrication due to sidewall roughness.MEMS: micro electro mechanical system
39 Deep Si etch - Bosch process Rough sidewall due to scalloping effect.1 cycle20 𝝁m deep pores
40 Chemical mechanical polishing (CMP) Pure physical polishing: low polish rate.Pure chemical reaction: cannot achieve smooth surface.The combination of the two provides efficient polishing.
42 Dual damascene process for IC interconnection bdcInitial layer structure.Two-step lithography to pattern both the trenches and via holes.Metal filling the trench and via holes by electroplating of Cu.Polish (CMP) back to make the surface flat for next level of interconnects patterningCuAl is replaced by Cu around year 2000 for IC interconnection due to Cu’s higher conductivity.Unlike Al, Cu is hard to etch by RIE, so CMP is adopted for the “dual damascene process”.
43 CMP of Cu interconnects for IC industry viatrenchVia-holes and trenches before Cu filling.CuSiO2Non-smooth surface after Cu plating into trench/via holes.Cu structure after removing dielectric materials.